Tables 361-367. 

 MAGNETIC PROPERTIES OF METALS. 



TABLE 361. - Cobalt at 100° 0. TABLE 362. -Nickel at 100° 0. 



321 



200 106 646 10650 54.2 



300 116 928 11960 39.9 



500 127 1016 13260 26.5 



700 131 1048 13870 19.8 



1000 134 1076 14520 14.5 



1500 138 1 104 15380 10.3 



2500 143 1 144 16870 6.7 



4000 145 1 164 18630 4.7 



6000 147 1 176 20780 3.5 



9000 149 1 192 239S0 2.6 



At 0° C. this specimen gave the fol- 

 lowing results : 



7900 I 154 I 1232 I 23380 I 3.0 



TABLE 363. - MagneUte. 



The following results are given by Du Bois * for a specimen of magnetite. 



Professor Ewing has investigated the effects of very intense fields on the induction in iron and other metals.t The 

 results show that the intensity of magnetization does not increase much in iron after the field has reached an in- 

 tensity of 1000 c. g. s. units, the increase of induction above this being almost the same as if the iron were not 

 there, that is to say, dBj dH is practically unity. For hard steels, and particularly manganese steels, much higher 

 forces are required to produce saturation. Hadfield's manganese steel seems to have nearly constant susceptibility 

 up to a magnetizing force of 10,000. The following tables, taken from Ewing's papers, illustrate the effects of 

 strong fields on iron and steel. The results for nickel and cobalt do not differ greatly from those given above. 



TABLE 364. — Lowmoor 

 Wrought Iron. 



TABLE 365. — Vicker's 

 Tool Steel. 



TABLE 366. — Hadlleld's 

 Manganese Steel. 



TABLE 367. —Saturation Values for Steels ol DlHerent Kinds. 



Bessemer steel containing about 0.4 per cent carbon . . . 

 Siemens-Marten steel containing about 0.5 per cent carbon 

 Crucible steel for making chisels, containing about 0.6 per 



cent carbon 



Finer quality of 3 containing about 0.8 per cent carbon . . 



Crucible steel containing I per cent carbon 



Whitworth's fluid-compressed steel 



H 



17600 

 18000 



19470 

 18330 

 19620 

 18700 



1770 

 1660 



1480 

 1580 

 1440 

 1590 



39880 

 38860 



38010 

 38190 

 37690 

 38710 



* " Phil. Mag." 5 series, vol. xxix, iSgo. 

 Smithsonian Tables. 



2.27 

 2.16 



1.95 

 2.08 

 1.92 



2.07 



t "Phil. Trans. Roy. Soc." 1885 and 1S89. 



